When we use the trivalent chromium blue zinc passivation solution, the galvanized workpiece can obtain a good bright blue appearance.However, sometimes yellow spots appear on the appearance of the workpiece after passivation, which seriously affects the appearance quality of the workpiece.Is this caused by improper use of trivalent chromium blue zinc passivation solution?
Bigolly Technology made an analysis based on the field experience and the characteristics of the product's trivalent chromium blue zinc passivation solution BZ-212,the phenomenon of yellow spots on the workpiece is not due to improper use of the blue zinc passivation solution. There are four main reasons:
1. Material problems of passivation tools.Some workpieces need to use a basket for passivation, but a stainless steel basket cannot be used as a passivation tool during passivation, it will affect the passivation effect of the workpiece, and a plastic basket should be used.
2, the structural problems of the workpiece.Some workpieces have blind holes, pits, welding gaps, etc., which are easy to hide water during passivation, resulting in yellow watermarks or spots after the workpiece is baked.During production, the water washing process should be improved according to the structural characteristics of the workpiece, and the residual water should be discharged as much as possible.
3. The water washing of the workpiece is poor.The workpiece may stick together during the washing process without good washing effect, resulting in yellow watermarks or spots on the surface of the workpiece.During production, the washing should be strengthened, or the washing time of the workpiece should be extended to ensure that the workpiece has a good washing effect.
4. The bright dipping of the workpiece is not good.After being used for many times, the bright dipping water is likely to become turbid due to a large number of impurities, which will affect the bright dipping effect of the workpiece. In particular, the cyanide-free alkaline galvanizing process is sensitive to impurities, and it is easy to appear macular phenomenon.During the production process, the bright dipping water should be replaced regularly, and the control of the bright dipping effect of the workpiece should be strengthened to ensure good bright dipping of the workpiece.
Therefore, the appearance of yellow spots after passivation of blue zinc workpieces is not due to improper use of trivalent chromium blue zinc passivation solution, but to check the material structure of the product itself, as well as the bright dipping and water washing processes.If you are interested in trivalent chrome blue zinc passivation solution,please contact Bigolly customer service to get free samples and detailed technical information!
If you want to know more about galvanizing, you can check "common problem".